#------------------------------------------------------------------------------
#$Date: 2019-11-17 08:34:46 +0200 (Sun, 17 Nov 2019) $
#$Revision: 228884 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/10/7231009.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7231009
loop_
_publ_author_name
'Clulow, Rebecca'
'Lightfoot, Philip'
_publ_section_title
;
 New sarcosine--metal halide complexes related to ferroelectric TSCC
;
_journal_issue                   28
_journal_name_full               CrystEngComm
_journal_page_first              4012
_journal_paper_doi               10.1039/C8CE00719E
_journal_volume                  20
_journal_year                    2018
_chemical_formula_moiety         'C9 H25 Mn N3 O8, 2(I)'
_chemical_formula_sum            'C9 H25 I2 Mn N3 O8'
_chemical_formula_weight         612.06
_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-05-03 deposited with the CCDC.
2018-06-25 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.8652(7)
_cell_length_b                   19.2670(15)
_cell_length_c                   10.3186(8)
_cell_measurement_reflns_used    857
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.5
_cell_measurement_theta_min      1.1
_cell_volume                     1961.3(3)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 13.6612
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Rigaku Mercury2 (2x2 bin mode)'
_diffrn_measurement_method       'profile data from ω-scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0978
_diffrn_reflns_av_unetI/netI     0.0436
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            19214
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.520
_diffrn_reflns_theta_min         2.114
_diffrn_source                   'Sealed Tube'
_exptl_absorpt_coefficient_mu    3.858
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.739
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'The program SADABS-2008/1 - G.M. Sheldrick was used to apply a multi-scan absorption correction.'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.073
_exptl_crystal_description       block
_exptl_crystal_F_000             1180
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.345
_refine_diff_density_min         -1.064
_refine_diff_density_rms         0.159
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.977
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     147
_refine_ls_number_reflns         2323
_refine_ls_number_restraints     5
_refine_ls_restrained_S_all      0.976
_refine_ls_R_factor_all          0.0916
_refine_ls_R_factor_gt           0.0421
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0585P)²+7.7627P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0964
_refine_ls_wR_factor_ref         0.1239
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1419
_reflns_number_total             2323
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c8ce00719e2.cif
_cod_data_source_block           shelx_CCDC6
_cod_depositor_comments
'Adding full bibliography for 7231003--7231021.cif.'
_cod_database_code               7231009
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, y+1/2, -z'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'-x-1/2, y-1/2, z-1/2'
'x, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
I1 I 0.01696(5) 0.40818(2) 0.74773(5) 0.04127(18) Uani 1 1 d . . .
Mn2 Mn 0.40838(13) 0.7500 0.78568(12) 0.0220(3) Uani 1 2 d S T P
O5 O 0.5198(4) 0.6681(2) 0.6802(4) 0.0298(10) Uani 1 1 d D . .
O2 O 0.0454(6) 0.7500 0.5463(6) 0.0310(15) Uani 1 2 d S T P
O3 O 0.2967(4) 0.6640(2) 0.8775(4) 0.0262(9) Uani 1 1 d . . .
O1 O 0.2435(6) 0.7500 0.6493(6) 0.0377(16) Uani 1 2 d S T P
C4 C 0.3422(6) 0.6046(3) 0.9036(6) 0.0263(14) Uani 1 1 d . . .
C1 C 0.1727(9) 0.7500 0.5492(9) 0.0245(19) Uani 1 2 d S T P
C2 C 0.2447(9) 0.7500 0.4213(9) 0.030(2) Uani 1 2 d S T P
N1 N 0.1496(8) 0.7500 0.3109(8) 0.0320(18) Uani 1 2 d DS T P
O4 O 0.4578(4) 0.5823(2) 0.8792(5) 0.0356(11) Uani 1 1 d . . .
C5 C 0.2433(6) 0.5550(3) 0.9680(6) 0.0277(14) Uani 1 1 d . . .
H5 H 0.2027 0.5777 1.0425 0.033 Uiso 1 1 calc R U .
H6 H 0.1713 0.5437 0.9076 0.033 Uiso 1 1 calc R U .
N2 N 0.3105(6) 0.4905(3) 1.0104(5) 0.0276(12) Uani 1 1 d D . .
C6 C 0.2185(7) 0.4408(4) 1.0766(7) 0.0373(17) Uani 1 1 d . . .
H9 H 0.1773 0.4630 1.1499 0.056 Uiso 1 1 calc R U .
H11 H 0.2695 0.4012 1.1052 0.056 Uiso 1 1 calc R U .
H10 H 0.1492 0.4260 1.0174 0.056 Uiso 1 1 calc R U .
C3 C 0.2142(15) 0.7500 0.1808(11) 0.043(3) Uani 1 2 d S T P
H1 H 0.299(9) 0.714(4) 0.417(8) 0.06(3) Uiso 1 1 d . . .
H2 H 0.088(8) 0.711(3) 0.304(9) 0.09(3) Uiso 1 1 d D . .
H3 H 0.269(9) 0.712(5) 0.175(9) 0.07(3) Uiso 1 1 d . . .
H4 H 0.152(13) 0.7500 0.126(12) 0.05(4) Uiso 1 2 d S . P
H7 H 0.376(5) 0.499(3) 1.077(4) 0.020(16) Uiso 1 1 d D . .
H8 H 0.358(6) 0.469(3) 0.940(5) 0.036(19) Uiso 1 1 d D . .
H12 H 0.519(16) 0.637(7) 0.755(10) 0.19(8) Uiso 1 1 d D . .
H13 H 0.610(3) 0.673(3) 0.646(6) 0.033(18) Uiso 1 1 d D . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Mn2 O2 168.8(2) . 6_657
O1 Mn2 O3 84.43(17) . .
O2 Mn2 O3 88.18(16) 6_657 .
O1 Mn2 O3 84.43(17) . 8_575
O2 Mn2 O3 88.18(16) 6_657 8_575
O3 Mn2 O3 97.5(2) . 8_575
O1 Mn2 O5 93.09(18) . 8_575
O2 Mn2 O5 94.76(17) 6_657 8_575
O3 Mn2 O5 175.79(18) . 8_575
O3 Mn2 O5 85.64(16) 8_575 8_575
O1 Mn2 O5 93.09(18) . .
O2 Mn2 O5 94.76(17) 6_657 .
O3 Mn2 O5 85.64(16) . .
O3 Mn2 O5 175.79(18) 8_575 .
O5 Mn2 O5 91.1(2) 8_575 .
C1 O2 Mn2 126.5(6) . 6_557
C4 O3 Mn2 126.7(4) . .
C1 O1 Mn2 164.9(6) . .
O4 C4 O3 126.6(6) . .
O4 C4 C5 117.4(6) . .
O3 C4 C5 115.9(5) . .
O1 C1 O2 125.5(9) . .
O1 C1 C2 117.7(8) . .
O2 C1 C2 116.9(8) . .
N1 C2 C1 112.3(7) . .
C2 N1 C3 115.2(8) . .
N2 C5 C4 111.8(5) . .
C5 N2 C6 113.9(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mn2 O1 2.151(6) .
Mn2 O2 2.199(6) 6_657
Mn2 O3 2.203(4) .
Mn2 O3 2.203(4) 8_575
Mn2 O5 2.209(5) 8_575
Mn2 O5 2.209(5) .
O2 C1 1.257(10) .
O2 Mn2 2.198(6) 6_557
O3 C4 1.260(7) .
O1 C1 1.246(11) .
C4 O4 1.244(7) .
C4 C5 1.518(9) .
C1 C2 1.499(13) .
C2 N1 1.476(12) .
N1 C3 1.486(13) .
C5 N2 1.476(8) .
N2 C6 1.486(8) .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N1 H2 I1 0.97(2) 2.58(3) 3.515(4) 164(8) 5_566
N2 H7 I1 0.96(2) 2.72(4) 3.565(6) 147(5) 2_565
N2 H8 I1 0.96(2) 2.75(2) 3.709(5) 174(5) 6_657
